Journal of Nanomaterials
Volume 2018 (2018), Article ID 4731970, 6 pages
https://doi.org/10.1155/2018/4731970

Research Article

Direct Synthesis of Highly Dispersible PACMA-Capped TiO₂ Nanoparticles and Its Adsorption Properties towards Pb(II)

Marta Sanchez-Sala,¹ Concepción Domingo,² and José A. Ayllón¹

¹Departament de Química, Universitat Autònoma de Barcelona, Campus UAB, 08193 Bellaterra, Spain
²Institut de Ciència dels Materials de Barcelona (CSIC), Campus UAB, 08193 Bellaterra, Spain

Correspondence should be addressed to José A. Ayllón; joseantonio.ayllon@uab.es

Received 12 July 2018; Accepted 28 October 2018; Published 19 December 2018

Academic Editor: P. Davide Cozzoli

Copyright © 2018 Marta Sanchez-Sala et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

A simple low-temperature one-step synthetic method of a hybrid material involving TiO₂ nanoparticles modified by an organic polymer is here reported. TiO₂ nanoparticles were grown by hydrolysis of hexafluorotitanate using boric acid as a fluoride scavenger. TiO₂ synthesis was performed in the presence of poly(acrylic acid-co-maleic acid) (PACMA). This procedure yields a crystalline TiO₂ nanopowder capped with PACMA, termed PACMA@TiO₂, according to X-ray diffraction and infrared spectroscopy characterization methods. Elemental analysis denotes the presence in the powder of a small amount of ammonium. Transmission and scanning electron microscopies show that the material is constituted by needles of ca. 200 nm in length, fused into star-like particles. Selected area electron diffraction analysis indicates that the particles are aggregated and only partially organized. The dried powdered material can easily be dispersed in water. The colloidal suspension obtained is highly stable, and its potential application in heavy metal adsorption is demonstrated with aqueous Pb(II), followed by using inductively coupled plasma optical emission spectrometry.

1. Introduction

Liquid phase deposition (LPD) is a wet process used for the formation of metal oxide thin films and powders at relatively low temperatures. The method is based on the hydrolysis of metallic fluorocomplexes and controlled by the addition of a fluoride scavenger, such as boric acid, which shifts the chemical equilibrium towards the precipitation of the corresponding metal oxide [1, 2]. LPD has been used to precipitate crystalline titanium dioxide (TiO₂) thin films homogeneously on different substrates. The method has been thoroughly studied by several groups, with special emphasis in determining factors that control nucleation and crystallinity [3–5]. This synthetic route allows the deposition of TiO₂ on labile organic substrates, for example, polyimide resins [6] and other polymeric films [7], since a thermal posttreatment is not required to produce crystalline materials. The deposition of hybrid TiO₂ films, incorporating compounds like alkylbenzene sulfonate surfactants [8] or copper phthalocyanine [9], is also feasible. In a different example, hybrid methylene blue/TiO₂ nanocomposite thin films have been used to fabricate light-activated oxygen indicators [10]. LPD has also been successfully used for the deposition of CNTs/TiO₂ composite films with photocatalytic activity [11]. Deki et al. have shown that the addition of polyethylene glycol during the growth of TiO₂ [12] or SnO₂ [13] by LPD allows the synthesis of monodisperse nanoparticles (3–5 nm). Likewise, polyvinylpyrrolidone has been used to tune the grain size of TiO₂ films deposited by LPD [14]. In all these examples, the used polymers are not incorporated to the final product, whereas in other examples, the adsorption of the polymer onto the oxide surface is a key factor to control the properties of the material. For instance, the addition of acrylic acid on the surface of TiO₂ nanoparticles increased the stability in water [15]. Methyl methacrylate has also been grown directly on the surface of 6-palmitate ascorbate-modified nanoparticles to make nanocomposites [16]. Inorganic nanoparticle-polymer hybrid composites have numerous applications [17]. An example is the formulation of easily processable dielectrics [18, 19] that usually require the modification of the oxide surface with coupling agents to favor their interaction with the polymer matrix, thus limiting nanoparticle aggregation [20]. Different polymers, including poly(acrylic acid) derivatives, are used to improve the stability of aqueous dispersions prior to deposition, as well as the adherence and homogeneity of deposited coatings [21, 22]. In these materials, the adsorbed polymer shell enhances nanoparticle dispersibility through steric and/or electrostatic effects. The adsorption properties are also modified.

In this work, poly(acrylic acid-co-maleic acid) (PACMA), a polyacid with great affinity to oxide nanoparticles improving its dispersibility [23, 24], was selected to control the growth of TiO₂ nanoparticles by LPD in a one-step route. The resulting end product, termed PACMA@TiO₂, precipitates in the form of nanopowder. Moreover, PACMA@TiO₂ is highly stable after water dispersion, which allows its use as a solid adsorbent for water pollutants. In this context, adsorption processes are being widely used by various researchers for the removal of heavy metals from waste streams. Indeed, pollution of water is a key problem worldwide, therefore optimizing processes that allow purifying industrial effluents very desirable. Specifically for Pb(II), the use of solid adsorbents for their elimination has many economic advantages [25]. It has been shown that pristine TiO₂ has some affinity for Pb(II) [26, 27], which can be improved by the control of particle morphology [28] and surface modification [29] or by using synergistic composites of TiO₂ and cellulose [30]. As a potential application, this study also analyzes the PACMA@TiO₂ adsorption of Pb(II) from the water.

2. Materials and Methods

2.1. Materials

Ammonium hexafluorotitanate (AHFT), boric acid, poly(acrylic acid-co-maleic acid) (PACMA, averaged molecular weight 3000 Dalton, 50 wt.% in H₂O), and Pb(II) nitrate were purchased from Sigma-Aldrich and used without further purification. Water purified with a Milli-Q system (Millipore, conductivity < 0.05 μS/cm) was employed.

2.2. Preparation of the PACMA@TiO₂ Powders

A solution of 660 mg of AHFT in 40 mL of water was mixed with another aqueous solution involving 623 mg of boric acid and 125 mg of PACMA in 40 mL. The mixture was a clear solution that resulted in a white precipitate after heating at 80°C for 3.5 h. The precipitate was separated by centrifugation, washed with fresh water, and dried at 60°C in an air oven. The estimated yield was 60%, considering that according to elemental analysis, the sample contains an 82 wt.% of TiO₂.

2.3. Characterization Techniques

Powder X-ray diffraction (PXRD) patterns were measured with a Siemens D5000 apparatus using the CuKα radiation. Patterns were recorded from 2θ = 5 to 50°, with a step scan of 0.02° counting for 1 s at each step. Sample morphology was observed with a scanning electron microscope (SEM) (Zeiss Merlin). Transmission electron microscopy (TEM) images were taken with a JEOL 2011 microscope operating at 200 kV. Selected area electron diffraction analysis was used to get information about crystallinity and aggregate order. The presence of adsorbed organics, including residual reagents, was ascertained by attenuated total reflectance Fourier-transform infrared (ATR-FTIR) spectroscopy (Bruker, Tensor model equipped with an MKII Golden Gate). Measurements of BET surface area were performed in a Micromeritics ASAP 2000 using low-temperature N₂ adsorption-desorption isotherms. Samples were previously degassed at 373 K during 18 h under vacuum. For UV-vis measurements, the powder was suspended in water aided by ultrasound and the spectrum was recorded over the wavelength range 200–800 nm using a Varian Cary UV-V spectrophotometer. DLS measurements were carried out in a Zetasizer Nano ZS (Malvern). Pollutant adsorption tests were performed in 50 mL aliquots taken from a mother solution containing 24 mg/L of Pb(II), prepared from Pb(NO₃)₂. Different amounts of PACMA@TiO₂ powder were added to these aliquots and left standing overnight. Stirring was not necessary to disperse the adsorbent. Finally, the different dispersions were centrifuged and each sample was analyzed using inductively coupled plasma optical emission spectrometry (ICP-OES, Optima 4300DV, Perkin Elmer) to determine the Pb(II) content.

3. Results and Discussion

LPD processes are mostly used to prepare thin films through heterogeneous nucleation on surfaces. In a different approach, in this work, the LPD route is used to obtain a fine precipitate. Homogeneous nucleation is enabled by the presence in the solution of a dissolved PACMA polymer, which has affinity to the growing TiO₂ crystallites. PACMA is thus adsorbed on the TiO₂ surface, discontinuing the growth and increasing the stability of the small nanometric particles in the aqueous growing media. Heterogeneous precipitation in the reactor walls was not observed. The precipitate was separated from the liquid phase by filtration before solid state characterization. The PXRD pattern recorded for the PACMA@TiO₂ sample matches that of the TiO₂ anatase phase (JCPDS no. 21-1272) (Figure 1). As usual in TiO₂ prepared by LPD, the relative intensity of the peaks indicates some preferential growth along the (004) direction. The widening in the low intensity peaks is due to the small crystal size, a fact that was confirmed by TEM characterization. TEM micrographs also showed the anisotropic shape of the precipitated nanoparticles in the form of needles. Primary crystals suffer some oriented agglomeration forming star-like macrostructures (Figure 2). The polycrystalline structure is also observed by selected area electron diffraction (insert in Figure 2), which displayed elongated spots arising from different Bragg reflections arising from individual needles fused together following some preferential crystal orientation. SEM pictures corroborate those observations (Figure 2). The star-like morphology would complicate the formation of compact aggregates. The estimated value of the BET surface area is 63 m²/g. The isotherm is type II (Figure 3), with a hysteresis H1 loop appearing at high relative pressure (>0.9), which is associated to pores created by agglomeration of uniformly sized particles.

Figure 1: Powder XRD pattern of a PACMA@TiO₂ sample. Anatase pattern was included for comparison (JCPDS no. 21-1272).

(a)

(b)

Figure 2: (a) TEM micrographs and associated SAED of PACMA@TiO₂. (b) SEM micrograph of a PACMA@TiO₂ sample.

Figure 3: N₂ gas adsorption-desorption isotherms of TiO₂@PACMA. The N₂ volume is at standard temperature and pressure (STP), and is the relative partial pressure of N₂ in equilibrium with the sample at 77 K.

ATR-FTIR spectrum (Figure 4) indicates that the material incorporates a small percentage of organic products (bands at 1715, 1630, and 1423 cm⁻¹). This behavior was expected considering that polycarboxylic acids have high affinity for the TiO₂ surface. The presence of two bands of different intensities assigned to asymmetric C=O stretching indicates that only some of the carboxylic acid groups are protonated (band at 1715 cm⁻¹), while most are deprotonated (band at 1630 cm⁻¹). The band at 1423 cm⁻¹ could be assigned to symmetric C=O stretching, but its position and relative intensity suggest that the sample contains also the NH₄⁺ cation adsorbed from the precursor solution. In fact, the broad absorption band around 3200–3100 cm⁻¹ is also compatible with the presence of NH₄⁺ cations (N-H stretching). Other contributions to this band are adsorbed water and the hydroxide anion. The measured elemental analysis (3.49% C; 1.57% H; 0.61% N) includes N in the composition, thus confirming the presence of residual ammonium in the composite, as it is the unique possible source of nitrogen. Additionally, elemental analysis results suggest the precipitation of PACMA@TiO₂ powder with a composition of 9 wt.% of polymer and a 9 wt.% of water, with one adsorbed ammonium each per three carboxylate groups. The percentage of water agrees with the weight loss measured during sample activation at 100°C under vacuum.

Figure 4: ATR-FTIR spectrum of PACMA@TiO₂ powder.

The obtained PACMA@TiO₂ solid powder was easily redispersed in water, and the obtained suspension was stable for weeks. In the synthetized product, the polymer coating provides both steric stabilization and charge stabilization of the nanoparticles. Dynamic light scattering characterization gave an averaged size of 200 nm for the dispersed powder (Figure 5), a value in accordance with SEM characterization. UV-vis spectra, obtained from the light transmitted through several aqueous suspensions of PACMA@TiO2 at different concentrations (Figure 6), showed the abrupt increase in the absorption below 380 nm typical of semiconductor crystalline TiO₂ [2].

Figure 5: Size distribution by the intensity of a TiO₂@PACMA sample redispersed in water.

Figure 6: Spectra obtained from the spectral measurement of light transmitted through a suspension of TiO₂@PACMA with a 1.0 cm optical path length at different concentrations.

As a potential application for the synthetized material as a solid adsorbent, its adsorption capacity was explored by choosing Pb(II) as a heavy metal pollutant to be removed from the water. The amount of Pb(II) adsorbed at equilibrium was determined in aqueous suspensions with different concentrations of PACMA@TiO₂. Any pH controlling additives were added. A 200 mg/L suspension of the composite was able to reduce the Pb(II) concentration from 24 to 3.5 ppm. This means that 100 mg of Pb(II) can be captured per gram of PACMA@TiO₂ adsorbent. By triplicating the amount of adsorbent in the aqueous dispersion, the quantity of Pb(II) remaining in the solution was reduced to less than 1 ppm. As a control, it was demonstrated that, under similar experimental conditions, 200 mg of commercial TiO₂ Degussa P25 adsorbed a significantly small amount of Pb(II), reducing the concentration from 24 to only 14 ppm. The adsorption results obtained with the PACMA@TiO₂ powder are comparable to others obtained with TiO₂ materials precipitated by much more intricate processes [25].

4. Conclusions

Polymer-functionalized TiO₂ nanoparticles were synthesized in a single step by LPD. The inorganic particles were capped with a partially deprotonated PACMA shell, with accompanying ammonium cations. The composite consisted of elongated particles of 200 nm that agglomerated in star-like macrostructures. The dried powder material was easily dispersible in water and can be used to adsorb remarkable amounts of Pb(II) from aqueous solutions, making it potentially valuable for environmental remediation applications.

Data Availability

Data used to support the findings of this study are included in the article.

Conflicts of Interest

The authors declare that there is no conflict of interest regarding the publication of this paper.

Acknowledgments

This work was partially financed by the Spanish National Plan of Research CTQ2014-56324-CO2-P1 and CTQ2017-83632 projects. C. D./ICMAB acknowledges the financial support from the Spanish MEC, through the “Severo Ochoa” Programme for Centres of Excellence in R&D (SEV-2015-0496). M. S-S. also acknowledges the Universitat Autònoma de Barcelona for his predoctoral grant.

References

S. Deki, Y. Aoi, O. Hiroi, and A. Kajinami, “Titanium (IV) oxide thin films prepared from aqueous solution,” Chemistry Letters, vol. 25, no. 6, pp. 433-434, 1996.

S. Deki and Y. Aoi, “Synthesis of metal oxide thin films by liquid-phase deposition method,” Journal of Materials Research, vol. 13, no. 04, pp. 883–890, 1998.

J. A. Ayllón, A. M. Peiró, L. Saadoun, E. Vigil, X. Domènech, and J. Peral, “Preparation of anatase powders from fluorine-complexedtitanium(IV) aqueous solution using microwave irradiation,” Journal of Materials Chemistry, vol. 10, no. 8, pp. 1911–1914, 2000.

H. Kishimoto, K. Takahama, N. Hashimoto, Y. Aoi, and S. Deki, “Photocatalytic activity of titanium oxide prepared by liquid phase deposition (LPD),” Journal of Materials Chemistry, vol. 8, no. 9, pp. 2019–2024, 1998.

T. P. Niesen and M. R. De Guire, “Review: deposition of ceramic thin films at low temperatures from aqueous solutions,” Solid State Ionics, vol. 151, no. 1-4, pp. 61–68, 2002.

H. Pizem, O. Gershevitz, Y. Goffer et al., “Titania deposition on PMR-15,” Chemistry of Materials, vol. 17, no. 12, pp. 3205–3213, 2005.

J. Ou, J. Wang, D. Zhang et al., “Fabrication and biocompatibility investigation of TiO₂ films on the polymer substrates obtained via a novel and versatile route,” Colloids and Surfaces B: Biointerfaces, vol. 76, no. 1, pp. 123–127, 2010.

L. Li, M. Mizuhata, and S. Deki, “Preparation and characterization of alkyl sulfate and alkylbenzene sulfonate surfactants/TiO₂ hybrid thin films by the liquid phase deposition (LPD) method,” Applied Surface Science, vol. 239, no. 3-4, pp. 292–301, 2005.

L. Li, M. Mizuhata, A. Kajinami, and S. Deki, “Different effects of alkyl sulfate and alkylbenzene sulfonate surfactants on the synthesis and properties of CuPc/TiO₂ composite films by the liquid-phase deposition (LPD) method,” Synthetic Metals, vol. 146, no. 1, pp. 17–27, 2004.

D. Gutiérrez-Tauste, X. Domènech, N. Casañ-Pastor, and J. A. Ayllón, “Characterization of methylene blue/TiO₂ hybrid thin films prepared by the liquid phase deposition (LPD) method: application for fabrication of light-activated colorimetric oxygen indicators,” Journal of Photochemistry and Photobiology A: Chemistry, vol. 187, no. 1, pp. 45–52, 2007.

Y. Wu, Z. Zhou, Y. Tuo et al., “A transparent CNTs/TiO₂ composite film with superhydrophobic and photocatalytic functions self-assembled by liquid-phase deposition,” Materials Chemistry and Physics, vol. 149-150, pp. 522–529, 2015.

S. Deki, A. Nakata, and M. Mizuhata, “High quality monodispersed oxide nanoparticles prepared by the liquid phase deposition method in aqueous polymer solution,” ECS Transactions, vol. 3, no. 9, pp. 29–35, 2006.

M. Mizuhata, Y. Umekage, A. Nakata, R. Kumaresan, and S. Deki, “Room-temperature synthesis of monodispersed SnO₂ nanoparticles by liquid phase deposition,” Chemistry Letters, vol. 38, no. 10, pp. 974-975, 2009.

M. Y. A. Rahman, A. A. Umar, L. Roza, and M. M. Salleh, “Morphological, optical, structural and photoelectrochemical properties of TiO₂ nanoflower prepared via PVP surfactant assisted liquid phase deposition technique,” Journal of Experimental Nanoscience, vol. 10, no. 12, pp. 925–936, 2015.

A. Solís-Gómez, M. G. Neira-Velázquez, J. Morales, M. A. Sánchez-Castillo, and E. Pérez, “Improving stability of TiO₂ particles in water by RF-plasma polymerization of poly(acrylic acid) on the particle surface,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 451, pp. 66–74, 2014.

E. Džunuzović, K. Jeremić, and J. M. Nedeljković, “In situ radical polymerization of methyl methacrylate in a solution of surface modified TiO₂ and nanoparticles,” European Polymer Journal, vol. 43, no. 9, pp. 3719–3726, 2007.

T. Hanemann and D. V. Szabó, “Polymer-nanoparticle composites: from synthesis to modern applications,” Materials, vol. 3, no. 6, pp. 3468–3517, 2010.

M. N. Tchoul, S. P. Fillery, H. Koerner et al., “Assemblies of titanium dioxide-polystyrene hybrid nanoparticles for dielectric applications,” Chemistry of Materials, vol. 22, no. 5, pp. 1749–1759, 2010.

D. N. McCarthy, H. Stoyanov, D. Rychkov, H. Ragusch, M. Melzer, and G. Kofod, “Increased permittivity nanocomposite dielectrics by controlled interfacial interactions,” Composites Science and Technology, vol. 72, no. 6, pp. 731–736, 2012.

T. Wang and J. L. Keddie, “Design and fabrication of colloidal polymer nanocomposites,” Advances in Colloid and Interface Science, vol. 147-148, pp. 319–332, 2009.

D. Schiemann, P. Alphonse, and P.-L. Taberna, “Synthesis of high surface area TiO₂ coatings on stainless steel by electrophoretic deposition,” Journal of Materials Research, vol. 28, no. 15, pp. 2023–2030, 2013.

S. H. Othman, S. Abdul Rashid, T. I. Mohd Ghazi, and N. Abdullah, “Dispersion and stabilization of photocatalytic TiO₂ nanoparticles in aqueous suspension for coatings applications,” Journal of Nanomaterials, vol. 2012, Article ID 718214, 10 pages, 2012.

I. Y. Tóth, E. Illés, R. A. Bauer et al., “Designed polyelectrolyte shell on magnetite nanocore for dilution-resistant biocompatible magnetic fluids,” Langmuir, vol. 28, no. 48, pp. 16638–16646, 2012.

J. Zhao, X. Wang, and L. Li, “Electrophoretic deposition of BaTiO₃ films from aqueous suspensions,” Materials Chemistry and Physics, vol. 99, no. 2-3, pp. 350–353, 2006.

A. M. López_Marzo, J. Pons, and A. Merkoçi, “Extremely fast and high Pb²⁺ removal capacity using a nanostructured hybrid material,” Journal of Materials Chemistry A, vol. 2, no. 23, pp. 8766–8772, 2014.

D. E. Giammar, C. J. Maus, and L. Xie, “Effects of particle size and crystalline phase on lead adsorption to titanium dioxide nanoparticles,” Environmental Engineering Science, vol. 24, no. 1, pp. 85–95, 2007.

M. S. Vohra and A. P. Davis, “Adsorption of Pb(II), NTA, and Pb(II)–NTA onto TiO₂,” Journal of Colloid and Interface Science, vol. 194, no. 1, pp. 59–67, 1997.

W. Zhao, I.-W. Chen, F. Xu, and F. Huang, “A novel ultralight three-dimensional house-of-cards titania monolith for extraordinary heavy-metal adsorption,” Journal of Materials Chemistry A, vol. 5, no. 30, pp. 15724–15729, 2017.

N. Pourreza, S. Rastegarzadeh, and A. Larki, “Simultaneous preconcentration of Cd(II), Cu(II) and Pb(II) on Nano-TiO₂ modified with 2-mercaptobenzothiazole prior to flame atomic absorption spectrometric determination,” Journal of Industrial and Engineering Chemistry, vol. 20, no. 5, pp. 2680–2686, 2014.

Y. Li, L. Cao, L. Li, and C. Yang, “In situ growing directional spindle TiO₂ nanocrystals on cellulose fibers for enhanced Pb²⁺ adsorption from water,” Journal of Hazardous Materials, vol. 289, pp. 140–148, 2015.